ZnO nanosheet arrays constructed on weaved titanium wire for CdS-sensitized solar cells
© Wu et al.; licensee Springer. 2014
Received: 23 January 2014
Accepted: 3 March 2014
Published: 11 March 2014
Ordered ZnO nanosheet arrays were grown on weaved titanium wires by a low-temperature hydrothermal method. CdS nanoparticles were deposited onto the ZnO nanosheet arrays using the successive ionic layer adsorption and reaction method to make a photoanode. Nanoparticle-sensitized solar cells were assembled using these CdS/ZnO nanostructured photoanodes, and their photovoltaic performance was studied systematically. The best light-to-electricity conversion efficiency was obtained to be 2.17% under 100 mW/cm2 illumination, and a remarkable short-circuit photocurrent density of approximately 20.1 mA/cm2 was recorded, which could attribute to the relatively direct pathways for transportation of electrons provided by ZnO nanosheet arrays as well as the direct contact between ZnO and weaved titanium wires. These results indicate that CdS/ZnO nanostructures on weaved titanium wires would open a novel possibility for applications of low-cost solar cells.
KeywordsZnO nanosheets CdS Nanoparticles Solar cells
Since the first work pioneered by O'Regan and Grätzel in 1991, dye-sensitized solar cells have been investigated extensively during the past two decades as promising alternatives to conventional silicon solar cells [1–5]. Although the light-to-electric conversion efficiency of 12%  reported recently was very impressive, the use of expensive and instability dyes to sensitize the solar cell is still not feasible for practical applications. Therefore, it is critical to tailor the materials to be not only cost-effective but also long lasting.
Narrow bandgap semiconductor nanoparticles, with unique bandgap characters, have been put forward as an efficient and promising alternative to ruthenium complexes or organic dyes in solar cell applications. Compared with conventional dyes, semiconductor nanoparticles have several advantages: (i) The large intrinsic dipole moments of the nanoparticles can lead to a large extinction coefficient and rapid charge separation, which is known to reduce the dark current and increase the overall efficiency. (ii) Because of their strong quantum confinement effect, the bandgap of semiconductor nanoparticles can be tuned by their sizes to match the solar spectrum. (iii) Furthermore, multiple exciton generation, where an electron with sufficiently high kinetic energy can generate one or more additional electron–hole pairs, has been predicted in semiconductor nanoparticles, providing new chances to utilize hot electrons or generate multiple charge carriers with a single photon. Hence, nanosized narrow bandgap semiconductor nanoparticles are promising light absorbers for solar cells to achieve improved performance.
A range of nanosized semiconductors, including CdSe [7–9], CdS [10–12], PbS [13, 14], and Cu2O , have been studied as sensitizers in place of conventional dye molecules for solar cell applications. For most of the reported nanostructured solar cells, transparent conductive oxide (TCO) glass is used as the substrate material. It is fragile, heavyweight, and a little high resistive, hampering its application in large-area solar cell modules. Recently, flexible solar cells, which are lightweight, portable, and economically cheap, have attracted significant academic interest and industrial attention. Indium tin oxide (ITO)- or fluorine-doped tin oxide (FTO)-coated polymer substrates are widely used as the substrate for flexible solar cells. However, the low temperature tolerance of those flexible plastic substrates limits the solar cell preparation process only below 200°C, resulting in a poor crystallization and photovoltaic performance. Metals with good flexibility, low resistance, high-temperature sinterability, and low cost are promising candidates as substrates in lightweight solar cells. Among the metals, Ti metal substrate, which has superior corrosion resistance to electrolytes in sensitized solar cells, has been studied by many groups [16–20]. It is expected that the application of weaved titanium wires as support of TiO2 or ZnO can not only reduce the weight of solar cell but also contribute to improve the performance of the solar cells by reducing internal resistance. However, most of the published works were based on conventional organic dyes; little work has been carried out on inorganic nanoparticles.
In this paper, ordered ZnO nanosheet arrays were grown on weaved titanium wires using a low-temperature hydrothermal method. By a successive ionic layer adsorption and reaction (SILAR) method, CdS nanoparticles were deposited onto the ZnO nanosheet arrays to fabricate CdS/ZnO nanostructures as a photoanode for a practical nanostructured solar cell. The effect of CdS SILAR cycles on the photovoltaic performance was studied systematically, and the optimized solar cells show a best light-to-electricity conversion efficiency of 2.17% with a short-circuit current density of 20.1 mA/cm2.
Preparation of ZnO nanosheets on titanium substrate
ZnO nanosheets were prepared by a two-step simple chemical solution method. In the first step, a layer of ZnO seeds was deposited onto weaved titanium wires by dipping the mesh in an alcohol solution containing 0.02 M zinc acetate dihydrate and 0.02 M lithium hydroxide, followed by annealing in a furnace at 400°C for 1 h. Then, the seeded substrate was placed into a glass bottle which contains an aqueous solution with 0.2 M of zinc nitrate and 1 M of urea. In the second step, the hydrothermal growth was conducted by heating the solution to 90°C for 12 h. After the hydrothermal treatment, the resultant nanostructure was rinsed with deionized water thoroughly and then annealed at 450°C for 1 h to remove any residual organics and convert into ZnO nanosheets.
Deposition of CdS nanoparticles with successive ionic layer adsorption and reaction method
CdS nanoparticles were deposited onto the ZnO nanosheet surface by SILAR method. Solutions of 0.05 M cadmium nitrate (Cd(NO3)2) and 0.05 M sodium sulfide (Na2S) were prepared by dissolving Cd(NO3)2 in deionized water and Na2S in methanol/water with volume ratios of 1:1. In a typical SILAR cycle, weaved titanium wire substrate, pre-grown with ZnO nanosheet arrays, was dipped into the Cd(NO3)2 aqueous solution for 30 s, rinsed in water, then dipped into the Na2S solution for another 30 s, and rinsed again in ethanol. This entire SILAR process was repeated to achieve the desired thickness of CdS nanoparticles. After the synthesis, the CdS/ZnO/Ti substrate was carefully washed in deionized water and dried at 100°C.
The morphologies of the ZnO/Ti and CdS/ZnO/Ti nanostructures were examined using a field-emission scanning electron microscope (FESEM; FEI Sirion, FEI Company, Hillsboro, OR, USA). The crystal structures of ZnO/Ti and CdS/ZnO/Ti were examined by X-ray diffraction (XRD; XD-3, PG Instruments Ltd., Beijing, China) with Cu Kα radiation (λ = 0.154 nm) at a scan rate of 2°/min. X-ray tube voltage and current were set at 40 kV and 30 mA, respectively. The optical transmission spectra were obtained using a dual-beam UV-visible spectrometer (TU-1900, PG Instruments Ltd., Beijing, China).
Solar cell assembly and performance measurement
The photovoltaic performance was characterized under an AM 1.5 G filter at 100 mW/cm2 using a Newport Oriel 94022A Solar Simulator (Model 94022A, Newport, OH, USA), as calibrated using a certified OSI standard silicon photodiode. A sourcemeter (2400, Keithley Instruments Inc., Cleveland, OH, USA) was used for electrical characterization during the measurements.
Results and discussion
Morphology and crystal structure of the nanostructured photoanodes
Optical property of the CdS nanoparticles
Photovoltaic performance of the solar cell based on CdS/ZnO/Ti nanostructures
V oc , J sc , FF, and efficiency
Our findings suggest the possible use of narrow bandgap semiconductor nanoparticles grown by simple SILAR method and inorganic semiconductor nanostructure material grown by a facile hydrothermal method for sensitized solar cell application. The CdS/ZnO nanostructures on weaved titanium wires can also be used as the photoanode in low-cost, flexible sensitized solar cells. In the present work, the power conversion efficiency of our solar cells was still not high enough for the practical applications. The rather poor fill factor is considered to be the main factor limiting the energy conversion efficiency. This low fill factor may be caused by the lower hole recovery rate of the polysulfide electrolyte, which leads to a higher probability for charge recombination . To further improve the efficiency of these nanosheet array solar cells, some new hole transport medium must be developed, one with suitable redox potential and low electron recombination at the semiconductor and electrolyte interface. Counter electrodes have also been reported to be another important factor influencing the energy conversion efficiency. Recently, a number of novel materials have been examined and tested as counter electrode materials; these studies prove the influence of various counter electrode materials on the fill factors of solar devices [22, 23]. Also, the open-circuit voltage can be further improved by using more efficient combination of semiconductor nanoparticles.
In summary, we have prepared CdS/ZnO nanostructures on weaved titanium wires by a hydrothermal treatment and a SILAR method. The resultant ZnO nanostructures consisted of a large number of well-aligned nanosheets, which are oriented vertically to the surface of titanium wires. This open-structured nanosheet array is beneficial to the deposition of CdS nanoparticles. An overall light-to-electricity conversion efficiency of 2.17% was achieved under 100 mW cm-2 illumination for the solar cells based on CdS/ZnO nanostructures with 20 CdS SILAR cycles. This results demonstrated that weaved titanium wires could be a valid alternative to classical FTO or ITO substrate with relatively low cost and satisfied internal resistance. In addition, the application of all inorganic semiconductors on weaved titanium wires may act as a novel architecture with lower cost and effective performance for further development of nanoparticle-sensitized solar cells.
This work was supported by the National Key Basic Research Program of China (2013CB922303, 2010CB833103), the National Natural Science Foundation of China (60976073, 11274201), the 111 Project (B13029), and the National Fund for Fostering Talents of Basic Science (J1103212).
- O'Regan B, Grätzel M: A low-cost, high-efficiency solar cell based on dye-sensitized colloidal TiO2 films. Nature 1991, 335: 737.View Article
- Gräzel M: Photoelectrochemical cells. Nature 2001, 414: 338. 10.1038/35104607View Article
- Kao MC, Chen HZ, Young SL, Lin CC, Kung CY: Structure and photovoltaic properties of ZnO nanowire for dye-sensitized solar cells. Nanoscale Res Lett 2012, 7: 260. 10.1186/1556-276X-7-260View Article
- Sun XM, Sun Q, Li Y, Sui LN, Dong LF: Effects of calcination treatment on the morphology and crystallinity, and photoelectric properties of all-solid-state dye-sensitized solar cells assembled by TiO2 nanorod arrays. Phys Chem Chem Phys 2013, 15: 18716. 10.1039/c3cp51941dView Article
- Zukalova M, Zukal A, Kavan L, Nazeeruddin MK, Liska P, Gratzel M: Organized mesoporous TiO2 films exhibiting greatly enhanced performance in dye-sensitized solar cells. Nano Lett 2005, 5: 1789. 10.1021/nl051401lView Article
- Yella A, Lee HW, Tsao HN, Yi C, Chandiran AK, Nazeeruddin MK, Diau EWG, Yeh CY, Zakeeruddin SM, Grätzel M: Porphyrin-sensitized solar cells with cobalt(II/III)-based redox electrolyte exceed 12 percent efficiency. Science 2011, 334: 629. 10.1126/science.1209688View Article
- Diguna LJ, Shen Q, Kobayashi J, Toyoda T: High efficiency of CdSe quantum-dot-sensitized TiO2 inverse opal solar cells. Appl Phy Lett 2007, 91: 023116. 10.1063/1.2757130View Article
- Liu LP, Wang GM, Li Y, Li Y, Zhang JZ: CdSe quantum dot-sensitized Au/TiO2 hybrid mesoporous films and their enhanced photoelectrochemical performance. Nano Res 2011, 4: 249–258. 10.1007/s12274-010-0076-7View Article
- Chen YX, Wei L, Zhang GH, Jiao J: Open structure ZnO/CdSe core/shell nanoneedle arrays for solar cells. Nanoscale Res Lett 2012, 7: 516. 10.1186/1556-276X-7-516View Article
- Wang CB, Jiang ZF, Wei L, Chen YX, Jiao J, Eastman M, Liu H: Photosensitization of TiO2 nanorods with CdS quantum dots for photovoltaic applications: a wet-chemical approach. Nano Energy 2012, 1: 440. 10.1016/j.nanoen.2012.02.005View Article
- Sun WT, Yu Y, Pan HY, Gao XF, Chen Q, Peng LM: CdS quantum dots sensitized TiO2 nanotube-array photoelectrodes. J Am Chem Soc 2008, 130: 1125.
- Kim J, Choi H, Nahm C, Moon J, Kim C, Nam S, Jung DR, Park B: The effect of a blocking layer on the photovoltaic performance in CdS quantum dot-sensitized solar cells. J Power Sources 2011, 196: 10526–10531. 10.1016/j.jpowsour.2011.08.052View Article
- Wang LD, Zhao DX, Su ZS, Shen DZ: Hybrid polymer/ZnO solar cells sensitized by PbS quantum dots. Nanoscale Res Lett 2012, 7: 106. 10.1186/1556-276X-7-106View Article
- Antonio B, Sixto G, Isabella C, Alberto V, Ivan M: Panchromatic sensitized solar cells based on metal sulfide quantum dots grown directly on nanostructured TiO2 electrodes. J Phys Chem Lett 2011, 2: 454. 10.1021/jz2000112View Article
- Liu YB, Zhou HB, Li JH, Chen HC, Li D, Zhou BX, Cai WM: Enhanced photoelectrochemical properties of Cu2O-loaded short TiO2 nanotube array electrode prepared by sonoelectrochemical deposition. Nano-Micro Lett 2010, 2: 277.View Article
- Dai H, Zhou Y, Chen L, Guo BL, Li AD, Liu JG, Yu T, Zou ZG: Porous ZnO nanosheet arrays constructed on weaved metal wire for flexible dye-sensitized solar cells. Nanoscale 2013, 5: 5102. 10.1039/c3nr34265dView Article
- Wu JH, Xiao YM, Tang JW, Yue GT, Lin JM, Huang ML, Huang YF, Fan LQ, Lan Z, Yin S, Sato T: A large-area light-weight dye-sensitized solar cell based on all titanium substrates with an efficiency of 6.69% outdoors. Adv Mater 2012, 24: 1884–1888. 10.1002/adma.201200003View Article
- Wang YH, Yang HX, Liu Y, Wang H, Shen H, Yan J, Xu HM: The use of Ti meshes with self-organized TiO2 nanotubes as photoanodes of all-Ti dye-sensitize solar cells. Prog Photovolt: Res Appl 2010, 18: 285–290.
- Onoda K, Ngamsinlapasathian S, Fujieda T, Yoshikawa S: The superiority of Ti plate as the substrate of dye-sensitized solar cells. Sol Energy Mater Sol Cells 2007, 91: 1176–1181. 10.1016/j.solmat.2006.12.017View Article
- Wang H, Liu Y, Huang H, Zhong MY, Shen H, Wang XH, Yang HX: Low resistance dye-sensitized solar cells based on all-titanium substrates using wires and sheets. Appl Surf Sci 2009, 255: 9020–9025. 10.1016/j.apsusc.2009.06.085View Article
- Lee YL, Chang CH: Efficient polysulfide electrolyte for CdS quantum dot sensitized solar cells. J Power Sources 2008, 185: 584. 10.1016/j.jpowsour.2008.07.014View Article
- Xu J, Yang X, Wong TL, Lee CS: Large-scale synthesis of Cu2SnS3 and Cu1.8S hierarchical microspheres as efficient counter electrode materials for quantum dot sensitized solar cells. Nanoscale 2012, 4: 6537. 10.1039/c2nr31724aView Article
- Burschka J, Brault V, Ahmad S, Breau L, Nazeeruddin MK, Marsan B, Zakeeruddin SM, Grätzel M: Influence of the counter electrode on the photovoltaic performance of dye-sensitized solar cells using a disulfide/thiolate redox electrolyte. Energy Environ Sci 2012, 5: 6089. 10.1039/c2ee03005eView Article
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.